Aircraft Manuf Materials(Composites)
Embed Size (px)
Transcript of Aircraft Manuf Materials(Composites)
Low-Cost Composite Materials and Structures for Aircraft ApplicationsDr. Ravi B. Deo Northrop Grumman Corporation Air Combat Systems, 9L10/W5 1 Hornet Way El Segundo, CA 90245, USA Dr. James H. Starnes, Jr. Mail Stop 190 NASA Langley Research Center Hampton, VA 23681, USA Richard C. Holzwarth AFRL/VASD, B45 Rm 118 2130 Eighth St Suite 1 WPAFB OH 45433-7542, USA
Abstract A survey of current applications of composite materials and structures in military, transport and General Aviation aircraft is resented to assess the maturity of composites technology, and the payoffs realized. The results of the survey show that performance requirements and the potential to reduce life cycle costs for military aircraft and direct operating costs for transport aircraft are the main reasons for the selection of composite materials for current aircraft applications. Initial acquisition costs of composite airframe components are affected by high material costs and complex certification tests which appear to discourage the widespread use of composite materials for aircraft applications. Material suppliers have performed very well to date in developing resin matrix and fiber systems for improved mechanical, durability and damage tolerance performance. The next challenge for material suppliers is to reduce material costs and to develop materials that are suitable for simplified and inexpensive manufacturing processes. The focus of airframe manufacturers should be on the development of structural designs that reduce assembly costs by the use of large-scale integration of airframe components with unitized structures and manufacturing processes that minimize excessive manual labor. Introduction The application of high performance composite materials to military aircraft can be traced back almost three decades to the F-14 (US Navy) and F-15 (US Air Force) fighters, which use boron/epoxy skins in their empennages. Since then the use of composite materials in military and transport aircraft has increased. Initial applications of composite materials to aircraft structures were in secondary structures such as fairings, small doors and control surfaces. As the technology matured, the use of composite materials for primary structures such as wings and fuselages has increased. A comprehensive list of current aircraft with a significant use of composite materials in the airframe is shown in Figure 1. As indicated in Reference 1, the aircraft industry chooses to use composite materials not only to reduce weight, but also because these materials are corrosion and fatigue resistant. The limiting factor in the widespread application of these materials has been their high cost compared to conventional metals. The
Paper presented at the RTO AVT Specialists Meeting on Low Cost Composite Structures, held in Loen, Norway, 7-11 May 2001, and published in RTO-MP-069(II).
application of composite materials for each of the aircraft listed in Figure 1 are reviewed in the present paper with respect to the following:
Fighter Aircraft (US) Fighter Aircraft (Europe) Fighter Aircraft (Russia) Bomber (US) Transport (US) Transport (US- Commercial) Transport (Airbus, European) General Aviation Rotary Aircraft
F-16, F-14, F-18,YF-23, F-22, JSF, UCAV Gripen JAS-39, Mirage 2000, Rafael, Eurofighter Typhoon, Lavi, DASA Mako MiG-29, Su series B-2 KC-135, C-17 KC- 135 B-777, B-767, MD-11 A-320, A-340, A380, Tu-204, ATR42, Falcon 900, A300-600 ST Piaggio, Starship, Premier 1 V-22, Eurocopter Tiger, Comanche RAH-66, Bell/Agusta BA-609, EH101, Super Lynx 300, S-92,
Figure 1. Aircraft composite materials usage surveyed.1. The typical weight fraction of composite structures in military, transport and general aviation aircraft 2. Factors influencing the use of composite materials 3. Payoffs associated with the applications reviewed 4. Factors limiting the use of composite materials 5. Technology developments in progress to remove the limitations 6. Potential role for composite materials in future airframes. The following paragraphs describe the results of this review. Combat Aircraft The trends in the use of composite materials for US Fighter aircraft are shown by three examples in Figure 2. The percentage by weight of composite materials used initially (e.g., F-15E) was small at 2%, but this percentage has since grown to more than 25% for the F-22 which is the designated replacement for the F-15E. The F-22 has demonstrated the feasibility and benefits of introducing processes such as RTM (Resin Transfer Molding) to improve the affordability of composite materials in combat aircraft applications. The use of composite materials in the US Navys F/A-18E/F equals nearly 20% of its structural weight in flight critical parts as shown in Figure 3. The choice of composite materials in the F/A-18E/F was dictated by a need to reduce weight and to improve strength, reliability and maintainability in an aircraft carrier environment. The center and aft fuselage skins and other ancillary structure, such as the speed brake and dorsal covers, are all-carbon/toughened- epoxy construction in the F/A-18E/F. Carbon fibers, such as Hexcels IM7, with improved strength and stiffness properties are used in the wing and the tail skins. Although composite materials in general are sensitive to impact damage, toughened materials such as Fiberites 977-3 toughened epoxy system used on the F/A-18E/F have successfully addressed this threat in operations. The AV-8B uses nearly 25% by weight of composite materials in its airframe.
49% 1987 32% 17% 2% 31% 21% 19% 29%
Aluminum Titanium Composites Other
39% 24% 21%
Figure 2. Materials usage trends in US fighter aircraft.
Percent of Structural Weight F/A-18C/D F/A-18E/F 31 49 Aluminum 14 15 Steel 21 13 Titanium 19 10 Carbon Epoxy 15 13 Other 100 100
Increased Carbon Epoxy Usage in Center and Aft Fuselage
Carbon Fibers (IM7) Used in Wing and Tail Skins
High Strength/Durability (AERMET 100) Used in and Flap Transmissions
Improved Toughness Resin (977-3) Used in All C/E Structural Applications
Figure 3. Materials distribution for the F-18 E/F aircraft.
The Eurofighter Typhoon is shown in a cutaway view in Figure 4, and uses composite materials in the wing skins, forward fuselage, flaperons and the rudder. Eurofighters exterior skins are made of Hexcels 8552 toughened epoxy and constitute 70% of the wetted area. Overall, 40% of the Eurofighters structural weight consists of carbon-fiber composite materials. The proportion of composite parts in Dassaults combat aircraft has grown steadily over the years, from 7 percent on the first Mirage 2000 fighters, to over 26 percent on the Rafale. Other fighters built by European companies such as the Saab Gripen, and EADS newly developed light fighter Mako use composite materials extensively in the 20-25% weight percent range.
Figure 4. Cutaway view of the Eurofighter Typhoon structure.The composites applications trend over the years in US and European combat aircraft is summarized in Figure 5. As shown in the figure, the composite fraction of the structural weight for fighter and attack aircraft seems to be leveling off at 30 percent. The payoff in combat aircraft is in performance in the form of reduced weight, increased payload and speed. Based on the prevalent applications seen by composites in combat aircraft, this limit is an indicator of lack of confidence in composite applications in highly 3-D loaded fuselage and wing substructures such as the main spars, and bulkheads e.g. the wing and landing gear attach bulkheads. Manufacturing and structural demonstration of innovative concepts in these areas is the next step if the 30 percent barrier is to be broken. Affordability is also a concern since costs associated with aircraft specific structural concept development, production implementation and recurring fabrication of complex composite parts with built in metal fittings and trunnions can exceed the $/lb saved ceiling for an aircraft. Therefore, cost reduction strategies for heavily loaded substructure need to be developed.
90 80 70 60 50 40 30 20Advanced Composites Content (% of Structural Weight)
Business Jets Commercial Bombers & Transports Fighters Rotors
F-22 A320 F-18E/F 777 B-1B C-17
Figure 5. Composite Application Trend in US and European Combat AircraftAnother feature to note in Figure 5 is the weight fraction of composites in the B-2, which seems to have broken the 30 percent barrier. This in spite of being a heavy lift class of aircraft where, as will be shown later, the limiting composites percent weight is even lower than for fighter/attack category of combat aircraft. Figure 6 illustrates the extent of carbon fiber and glass fiber composites usage on the B-2 that results in the high weight fraction. For the B-2, stealth or minimizing the radar cross-section was the primary driver and as such carbon fiber composites were extensively used in the primary structure to offset the weight penalty from radar absorbing materials applied to the exterior. Due to the lower density of composites compared to metals, the volume fraction of the airframe that is composite is considerable and may exceed 60 percent. Of special note in the case of the B-2 is that stealth performance requirements dictate significantly increased usage of composites.
Fixed Trailing Edge
Aft / Center Wing Assembly